Rapid Tooling for Plastic Injection Moulding Using ... falves/ · PDF file Rapid Tooling...
Embed Size (px)
Transcript of Rapid Tooling for Plastic Injection Moulding Using ... falves/ · PDF file Rapid Tooling...
Rapid Tooling for Plastic Injection Moulding Using Indirect Rapid Tooling Processes
F. Jorge Lino, Pedro V. Vasconcelos, Ricardo Paiva and Rui J. Neto
INEGI, Instituto de Engenharia Mecânica e Gestão Industrial, Rua do Barroco, 174, 4465-591 Leça do Balio, Portugal, Tel.: (351) 229578710, Fax: (351)
229537352, firstname.lastname@example.org, www.fe.up.pt/~falves
Abstract: Rapid Prototyping (RP) and Rapid Tooling (RT) are well known processes
for rapidly develop new products and consequently reduce the time to market. In Portugal, many companies are still not exploring the full advantages of using these technologies for new products development and produce reduced runs. This work presents some results obtained with composite tools manufactured for thermoplastics injection. These tools are obtained by casting a aluminium filled resin or by arc spray metal tooling over Rapid Prototyping models. Different properties, such as: moulds roughness, hardness and the wear were determined and compared, and the suitability of these processes are evaluated to rapidly produce prototype moulds to inject thermoplastic models and pre series.
Introduction: RP and RT systems are used to reduce product development time, schedules
and deadlines. This way the companies are able to deliver new products in less time, with greater quality at lower expenses. Two categories of RT exist; a direct approach, where the RP machine builds the actual tooling inserts (examples of these processes are the DMLS, SLSm, ProMetal, LENS, etc.), and an indirect category, where a RP master pattern is used to produce a mould.
Currently, there is an increase interest in RT solutions. Whether the application is prototype, bridge, or short-run production, RT represents an excellent opportunity to reduce both time and expense. Methods of RT are relatively new, and some are still in development all around the world.
The production of prototypes moulds in silicone, polyurethane and epoxy resins, allow the production of dozens to hundreds parts for visual aids, geometric and dimensional analysis, and frequently thermoplastic functional prototypes or pre series. Particularly, for these last functional prototypes, epoxy based composites can be used to manufacture the injection moulds for thermoplastics. These types of moulds can withstand the high pressures and
temperatures of the thermoplastic injection cycle. Naturally, their expected life lies between 100 and 1000 cycles which are significantly lower than the ones obtained with the conventional metallic moulds that are more expensive and time consuming and require intensive machining operations. Considering that the development of an industrial product rarely demands a higher number of prototypes, it can be concluded that these technologies are very attractive and well adjusted for rapid development of new products, reducing the time to market and increasing the companies’ competitiveness [1-5].
Fig. 1 shows one epoxy based composite mould that was used in the production of a thermoplastic part included in functional prototypes of a terminal of an automatic teller machine. Fig. 2 presents other composite mould and a pre series of a latch.
a) b) c)
Fig. 1 - New products development using composite moulds: a) ABS prototype model obtained by High Speed Machining (HSM) and used as a master to produce the composite mould; b) composite mould in aluminium filled resin; c) final component with the thermoplastic injected part.
a) b) c)
Fig. 2 - Epoxy based composite mould for thermoplastic injection of a latch: a) composite mould; b) preparation of the core and cavity in the standard plate of an industrial injection machine; c) pre series of the latch.
The composite moulds based on high temperature epoxy resins, used in rapid tooling, exhibit an intermediate durability between the soft and the hard tooling [2-4]. This is due to the combination of the high strength and good thermal stability of the epoxy resin, with the stiffness, hardness and good thermal conductivity of the metallic particles. This last characteristic reduces the thermal shock in the mould in each injection cycle, lowering the mould temperature and the injection cycle time.
Although this technology seems to be considered for pre series production of
thermoplastic parts, difficulties related with the brittleness, size, erosion and the reduced thermal conductivity of the mould, limits their more popular use. Considering this limitation, our research group has been working in a complementary solution using sprayed-metal prototype moulds. These moulds are obtained by depositing an outside layer of a zinc-based alloy (kirksite type) over RP models, followed by a casting of a low cost backup of aluminium filled polyurethane resin (epoxy or acrylic resins can also be used). This low cost resin (cheaper than the high temperature epoxy resin used in the composite moulds) makes this process very attractive to produce large parts. It is expected to achieve with these moulds a slight improvement in the heat dissipation capacity (lower cooling cycles), better mechanical resistance and accuracy (the mould- making process introduces little or no additional shrink).
The implementation of the two indirect rapid tooling processes to
manufacture prototype moulds for production of functional prototypes and pre series, with reduced costs and reduced time-to-market, will allow Portuguese companies, that have a larger tradition in manufacturing moulds for thermoplastic injection industry, to increase their competitiveness in a continuous more demanding international market [5, 6-8].
Two types of moulds were manufactured by indirect rapid tooling: 1. Composite moulds; 2. Sprayed-metal moulds.
Composite Moulds Aluminium filled composites, with different aluminium particles
concentrations (AF), and hybrid composites composed by aluminium particles and milled fibres (AFV) were produced (see table 1). In previous work [9-11],
the authors studied different resin formulations and curing cycles and end-up with these two most promising compositions for this indirect rapid tooling application. The respective microstructures of the two types of composites are presented in fig. 3. The epoxy matrix system composition is indicated in table 2, and the technical characteristics of the dispersed materials presented in table 3.
Fig. 4 shows the main steps of the technique used to cast the composite resins . This procedure assures composite moulds with low level of porosity.
Table 1 – Designation and composition (in volume %) of the materials produced.
Epoxy resin Aluminium filled composite Hybrid composite A
A – 100% AF
A – 59 % F – 41 %
AGF A – 57.5 %
F – 38.5 %, G – 4 % A – Epoxy resin; F – Aluminium particles; G – Glass milled fibres
a) b) Fig. 3 - Epoxy resin composites filled with: a) aluminium (grey round particles); b) aluminium and milled glass fibres (dark elongated filaments).
Table 2 - Epoxy system composition.
Epoxy system Araldite LY5210/
Aradur HY2954 (Vantico-USA)
Epoxy components ● TGDDM = N, N, N´, N´- tetraglycidyl – 4, 4´ - diaminodifenylmethane ● butahedioldiglycidyl ether
Curing agent ●2, 2’-dimetil-4, 4’-metilenobis (ciclohexilamine)
Table 3 - Technical characteristics of the aluminium particles and milled fibres.
Fibre type Manufacturer Dimensions Sizing Aluminium particles
(>99% Al) Hexcel (France) P200 degree -
Glass fibres PPG (USA) 215/11µm (l/d)* Polyvinyl acetate with silane
Carbon fibres Toray (Japan) 63/7µm (l/d)* 1 wt% epoxy
*l/d – fibre length/diameter.
Fig.4 - Processing method using vacuum pouring: a) manual component mixture; b) first degassing; c) second degassing with agitation; d) vacuum pouring.
The processing conditions, dimensional changes occurring during the
process, mechanical and wear resistance with the temperature, and the thermal conductivity, were studied with detail, aiming to produce moulds with optimised properties for thermoplastic injection.
After tested and characterized in laboratory, the two composite moulds (cost
of the mixture is 13.5/kg) were applied in an industrial thermoplastic injection machine for tests.
Sprayed-Metal Moulds After the CAD design of the part to be manufactured, the STL file was sent
to a Rapid Prototyping machine (stereolitography VIPERsi2, 3D Systems, USA),
and the SL model produced. It should be mentioned that although a SL model was used for this part, other types of RP models, such as LOM (paper models) could be employed, due to the fact that during an adequate metallic projection, the maximum temperature reached by the shell is lower than 50ºC .
The RP model was placed in a support structure that defines the parting surface, mounted in wood box and manually coated (using a brush) with a thin layer of a release agent fluid (polyvinyl alcohol - PVA, MCP HEK Tooling, Germany) (fig. 5a). It should be mentioned that the support structure can be modelled using CAD 3D systems, and also manufactured using RP technologies.
a) b) Fig. 5 - Arc spray metal tooling: a) wood box containing the stereolitography R